Bone Tissue Mechanics

Transcrição

Bone Tissue Mechanics
```Bone Tissue Mechanics
Paulo R. Fernandes
Instituto Superior Técnico, 2013
PART 6
Biomecânica dos Tecidos, MEBiom, IST
Fatigue
Biomecânica dos Tecidos, MEBiom, IST
Fatigue – damage accumulation. The failure occurs even for load
below the failure stress.
low number of cycles (< 103 ; σ > σy )
Fatigue Analysis
high number of cycles (> 103 ; σ < σy )
fracture mechanics – crack propagation
Biomecânica dos Tecidos, MEBiom, IST
Fatigue for a high number of cycles:
Biomecânica dos Tecidos, MEBiom, IST
S-N curve (adjusted for experimental data):
When
Curve of the type:
Biomecânica dos Tecidos, MEBiom, IST
Effect of σm
Alteration
Substituing
by
Goodman Relation (empirical)
Biomecânica dos Tecidos, MEBiom, IST
Problem
A beam is used to lift containers. Knowing that the weight of each container is
P=356 kN and that the maximum bending moment is Mmax=PL/8, determine the
life-time for the beam if the beam works 200 days per year and it lifts 20
containers per day.
Beam properties
Material properties
Biomecânica dos Tecidos, MEBiom, IST
Solution:
min
min
Biomecânica dos Tecidos, MEBiom, IST
Number of cycles:
Number of cycles/year:
cycles/day
cycles/year
days/year
cycles
cycles/year
years
years
Biomecânica dos Tecidos, MEBiom, IST
Fracture mechanics
Crack propagation
Biomecânica dos Tecidos, MEBiom, IST
Introduction to linear elastic fracture mechanics
Biomecânica dos Tecidos, MEBiom, IST
Introduction to linear elastic fracture mechanics
• The state of stress at the crack tip is complex
σ
Crack
dimension
a
(nominal stress)
• The analysis is based on the stress intensity
factor K
β is a parameter that depends on geometry and
The unit for K is
• Fracture occurs if the stress intensity factor K is
higher then the material Kc (fracture toughness)
Biomecânica dos Tecidos, MEBiom, IST
Example
data
thickness
Steel
Steel
a) For the material type C, determine the value of failure load P ?
b) If the same load is applied to the material D, what is the critical crack length?
Biomecânica dos Tecidos, MEBiom, IST
Solution:
critical situation
nominal stress
nominal stress:
Biomecânica dos Tecidos, MEBiom, IST
critical situation
unknown
Data:
Solving the equation:
Biomecânica dos Tecidos, MEBiom, IST
Crack propagation analysis
Biomecânica dos Tecidos, MEBiom, IST
Crack propagation
For cyclic loads cracks propagate for values of
K < Kc
Biomecânica dos Tecidos, MEBiom, IST
Problem
-A cylinder with a diameter of 12,7 mm is subject to an alternating tension
load between 0 and 44,5 kN.
- the cylinder has a crack with initial length of a0 = 0,254 mm
- the material property is
- the parameter to apply the Paris Law are: A= 19,1x10-12 and n=3.
How many cycles are needed to reach failure?
Biomecânica dos Tecidos, MEBiom, IST
Solution
The alternating stress is:
ΔK is:
The critical length of the crack ac is:
Biomecânica dos Tecidos, MEBiom, IST
The number of cycles to reach failure is:
Paris Law
thousand cycles
Biomecânica dos Tecidos, MEBiom, IST
Fatigue and Fracture Resistance
of Bone
Biomecânica dos Tecidos, MEBiom, IST
Bone Failure – Fatigue and Creep
• bone does not fail only under loads large enough to exceed the failure
stress (monotonic fracture).
• different loads, corresponding to stress below the failure stress, can lead to
• There are two ways for this failure, fatigue and creep (sometimes working
together)
• fatigue is the result of cyclic loads (that not exceed the failure stress)
• in creep the load is applied continuously (not exceeding the failure
stress).
t=0
t=0+
t»0
F
F
Biomecânica dos Tecidos, MEBiom, IST
damage – micro cracks
Biomecânica dos Tecidos, MEBiom, IST
damage – micro cracks
• damage due to fatigue/creep can be observed in
healthy bones, in the form of microcracks.
• these microcracks can, under certain conditions,
growth in number, as well as growth in length and
become macrocracks that can lead to bone failure.
• in general, these microcracks are removed by bone
remodeling.
• when the damage accumulation is faster then bone
remodeling a “stress fracture” can occur. (elite
athletes, soldiers, ballet dancers, etc…)
• the crack propagation is also controlled by the lamellar structure of bone.
• can be also some congenital defect or introduced during a surgical procedure.
Biomecânica dos Tecidos, MEBiom, IST
damage – micro cracks
• the damage accumulates exponentially, and more
rapidly in woman than in men, after the 40 years old.
• Burr and Stafford (1990) counted 0.014
microcracks /mm2 in the ribs of a 60 years-old man.
• Wenzel et al. (1996) found approximately 5
microcracks/mm2 in the trabecular bone from the
spine.
•About 80%−90% of micro cracks in cortical bone
are found in the interstitial matrix between osteons,
with a dimension of 50-100 μm.
Biomecânica dos Tecidos, MEBiom, IST
The effect of age in microdamage
• the evolution of microcracks with age is
exponential .
• after the 40 year-old the crack density is
higher in woman.
• probably this is related with the reduction
of bone mass, increasing bone strain, and
probably fatigue damage is sensitive to the
strain magnitude.
• many nontraumatic fractures in the
elderly (osteoporotic fractures) are
essentially stress fractures.
• remember the BMU activation with age,
namely after 40 years old (is there any
relation?)
Biomecânica dos Tecidos, MEBiom, IST
Fracture mechanics – introduction
Linear elastic fracture
mechanics, G.R. Irwin (1957)
• to measure the severity of a crack the stress intensity
factor K is used,
K = C.s.(π.a) ½
[K]=MPa.m½
where s is the nominal stress, a is the crack length and
C is a coefficient related with the crack geometry and
• 3 different kinds (modes) of cracks:
Mode I – tension
Mode II - shear
Mode III – tearing
Biomecânica dos Tecidos, MEBiom, IST
Fracture mechanics – introduction
• if for a given load the stress intensity factor, K, is greater than a critical
value, Kc (the values supported by the material) then the crack will
propagate.
• the maximum value support by the material (critical value), Kc, is the
fracture toughness.
• note the low fracture
thougness of bone
cement (PMMA)
Biomecânica dos Tecidos, MEBiom, IST
Fracture mechanics – introduction
• cracks in long bones propagate in a direction
parallel to the bone axis.
• when a crack propagates transversally
(perpendicular to lamellar structure) the crack
tends to change the direction and propagate along
the principal axis of the bone.
• the fracture toughness of bone is anisotropic .
Biomecânica dos Tecidos, MEBiom, IST
Fracture mechanics – introduction
Example:
• for a human tibia, KIc=4 MPa.m½
• for a circular crack with radius a on the tension surface of a long bone under
bending, the stress intensity factor KI can be approximated by,
KI = 2×1.025.s.(a/π) ½
• assuming for the elastic modulus E=20 GPa and for strain ε=2000 με (it is a
physiologic strain level), the applied stress is:
s = E.ε = 20×109 × 2000×10−6 = 40 MPa
• KI = KIc  2× 1.025.s.(ac /π) ½ = KIc  2× 1.025 × 40 × (ac / π) ½ = 4
 ac = [4 / (2× 1.025 × 40)]2 × π
 ac = 7.5 mm
• so, the critical length for the crack is ac = 7.5 mm, that is a very high value.
Biomecânica dos Tecidos, MEBiom, IST
Fatigue behavior of bone –S-N curve
• the bone behavior to cyclic loads is analog to other materials used in engineering – the
fatigue process diminish the elastic modulus. The logarithm of the fatigue life (number of
cycles until failure) is linearly proportional to the logarithm of stress (alternating stress)
and cracks appears resulting from fatigue damage.
• NF=c / Sq, where c is a coefficient and q is
a number between 5 and 15 depending on the
•For the human femur (cortex) unden uniaxial
tension → NF = 1.445×1053 / S14.1
compression → NF = 9.333×1040 / S10.3
where S is normalized by the initial elastic
modulus. Thus S is also a strain and the units is με.
• These data was obtain for superphysiologic strain
(2600−6600 με).
• Extrapolating for physiologic levels of strain
(2000 με) the fatigue life would be 4.1 millions of
cycles in tension and 9.3 millions in compression.
Biomecânica dos Tecidos, MEBiom, IST
Fatigue behavior of bone – compression vs tension
• also the type of cracks is different in
tension and in compression.
• in tension the cracks are placed in the
interstitial space of the cortical bone.
•In compression crack tends to go from a
Havers canal to another Havers canal .
Biomecânica dos Tecidos, MEBiom, IST
Fatigue and bone remodeling
• the main function of remodeling is to renew bone,
namely removing the fatigue damage.
• It has been estimated that the bone turnover and the
fatigue live are related, i.e, the period of bone turn
over coincide with the estimated fatigue life.
• there are theories saying that cracks break the
osteocytic network, inhibiting the communication
between osteocytes and originate the process of bone
remodeling.
• several studies conclude that there an intense
remodeling activity when the quantity of cracks is
bigger.
ulna rats, which do not ordinary remodel their
cortical bone, they were able to demonstrate
microcracks in association with BMU resorption
cavities.
Biomecânica dos Tecidos, MEBiom, IST
Bibliography
 Skeletal Tissue Mechanics , R. Bruce Martin, David B. Burr, Neil A.
Sharkey, Springer Verlag,1998.
Musculeskeletal Systems, D. Bartel, D. Davy, T. Keaveny, Pearson
Prentice Hall, 2006.
 Bone Mechanics Handbook, 2nd Edition, S.C. Cowin, CRC Press,
2001
 Mechanics of Materials, 5th Edition, F. Beer, Jr., E. R. Johnston , J.
DeWolf, D. Mazurek, McGraw Hill, 2009
Biomecânica dos Tecidos, MEBiom, IST
```

Bone Tissue Mechanics

•Basically loads are transmitted by joint, so the question is how to know the forces in joints. •It is possible to obtain an order of magnitude of this loads using free body diagrams and static ana...

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais

Leia mais